Abstract
Higher order topological insulators (HOTIs) are a new class of topological materials which host protected states at the corners or hinges of a crystal. HOTIs provide an intriguing alternative platform for helical and chiral edge states and Majorana modes, but there are very few known materials in this class. Recent studies have proposed Bi as a potential HOTI, however, its topological classification is not yet well accepted. In this work, we show that the (110) facets of Bi and BiSb alloys can be used to unequivocally establish the topology of these systems. Bi and Bi_{0.92}Sb_{0.08} (110) films were grown on silicon substrates using molecular beam epitaxy and studied by scanning tunneling spectroscopy. The surfaces manifest rectangular islands which show localized hinge states on three out of the four edges, consistent with the theory for the HOTI phase. This establishes Bi and Bi_{0.92}Sb_{0.08} as HOTIs, and raises questions about the topological classification of the full family of Bi_{x}Sb_{1−x} alloys.
Similar content being viewed by others
Introduction
HOTIs are topological crystalline insulators that have protected topological features on the boundaries with codimension greater than one. In contrast to (1st order), threedimensional timereversal protected topological insulators that show an insulating bulk with conducting surface modes, threedimensional 2nd order HOTIs show insulating bulk and surfaces, but with onedimensional conducting channels at hinges (i.e., the intersection of two surface facets) or equivalent crystal defects^{1,2,3,4,5,6}. While several groups have recently succeeded in observing HOTI phases in an electronic circuit, phononic, and photonic systems^{7,8,9,10}, the experimental realization and characterization of HOTIs in solidstate materials has proven more challenging. Among the proposed HOTI materials^{4,11,12,13,14,15,16}, bulk Bi has recently emerged as a key candidate. Bi and Bi_{1−x}Sb_{x} alloys are wellknown important topological materials with highly tunable electronic properties. Scanning tunneling microscopy studies^{1,17} have observed signatures of onedimensional modes on the edges of (111) facets of Bi, but the higherorder topological origin of these edge modes remains to be unequivocally established. Indeed an earlier study modeled the (111) facet as a freestanding Bibilayer^{17}, which is predicted to be a quantum spin Hall insulator, and hence attributed the observed hinge modes to edge states of a quantum spin Hall system. In contrast, a recent study^{1} ascribed the metallic edge modes to the manifestation of a bulk HOTI protected by crystalline and timereversal symmetries. New experimental data is necessary to distinguish between these scenarios. Importantly, the confirmation of Bi as a HOTI would indicate that the lowenergy bands of bismuth must have trivial timereversal protected \({{\mathbb{Z}}}_{2}\) topology^{1,18}. This not only has implications for the topology of bulk Bi, which still remains controversial, but also the family of Bi_{1−x}Sb_{x} alloys.
Results
STM measurements on Bi and Bi_{0.92}Sb_{0.08} films
Bi naturally cleaves along the (111) plane, which makes STM studies of other planes, e.g., (110), difficult in bulk cleaved crystals. To circumvent this problem, we use molecular beam epitaxy (MBE) to grow Bi and Bi_{0.92}Sb_{0.08} films on ndoped silicon (111) wafers^{19,20,21,22,23}. The films were grown in a custom MBE system (described in more detail in the “Methods” section), and the composition was confirmed using Rutherford backscattering spectrometry (see Supplementary Note 4). Film thicknesses were chosen to be in the range of 30–90 bilayers (BLs) to ensure that they are representative of the bulk.
To establish a benchmark for comparison, we first reproduce the edge state data previously obtained on Bi(111) crystals using our films. STM topographies on our Bi(111)/Si(111) films reveal triangular islands and a hexagonal lattice indicative of (111) facets. The dI/dV spectra on the bulk and edges of the triangular islands show signatures of the Van Hove singularity associated with the surface states, as well as the emergence of clear 1D modes at typeA edges (see Supplementary Note 1), as was observed in the cleaved bulk Bi crystals^{17}. Having confirmed the presence of edge modes in the (111) films, we move on to the (110) films.
By changing the growth conditions (see “Methods” section), we were able to grow Bi and Bi_{0.92}Sb_{0.08} in the (110) orientation on the same Si(111) substrates. STM images of the (110) oriented films of both Bi and Bi_{0.92}Sb_{0.08} are shown in Fig. 1. Large area topographic images of bismuth films (Fig. 1b) show that the surface is uniformly covered with (110) oriented rectangular islands with longer edges parallel to the (\(1\bar{1}0\)) direction. Figure 1e shows an STM image with its corresponding Fourier transform in the inset. Height profiles along line cuts (red and blue color lines in Fig. 1e) confirm the lattice constants of the pseudocubic crystal structure of Bi(110), i.e., 0.443 and 0.471 nm in Fig. 1g, h, respectively. Representative spectra at the center of the Bi and Bi_{0.92}Sb_{0.08} (110) islands, shown in Fig. 1i, j, reveal a broad increase in the density of states (DOS) above 130 mV in both samples. This increase can be ascribed to the spinsplit Rashba surface states known to exist in bismuth and its alloys^{19,24}.
Spectroscopic measurements on a rectangular facet of Bi(110)
We first focus on the edge states observed on rectangular islands of the Bi (110) films. Spectra on the edge of the islands show a sharp peak in the DOS as shown in Fig. 2c. This singularity corresponds to bound modes which are localized within a few nanometers of the edge, as seen in the spectroscopic measurements across and along the edge shown in Fig. 2d, e respectively. This sharp peak resembles the DOS feature observed on the edges of Bi(111). To further characterize this edge mode, we obtain spectroscopic data on all four edges of a (110) oriented rectangular island as shown in Fig. 3b, c, d, and e. Intriguingly we find that only three out of four edges show clear edge modes, while the fourth edge shows no peaks. We confirmed this observation by measurements on different rectangular facet islands on multiple samples. In all cases, the edge that shows no edge modes is the one that is perpendicular to the (\(1\bar{1}0\)) direction. Crucially, the observation of edge states on three out of the four edges cannot be attributed to different bonding on just one side, which was a key part of the argument in ref. ^{17}. By looking at the lattice structure of the (110) facet, we know that the two short sides are identical from a bonding perspective (see Supplementary Note 6). Yet, for a given island, one short side shows hinge states while the other does not.
Theoretical justification
To understand the novel pattern of rectangular island edge modes on the (110) facets, let us first briefly review the recent developments for the topology of bismuth. Specifically, refs. ^{1,18} argued that the bulk topology of bismuth can be described as two copies of a strong 3D TI, i.e., twoband inversions at the Tpoint. Since there is an even number of strong TI copies, they conclude that the lowenergy bulk bands of bismuth have trivial strong \({{\mathbb{Z}}}_{2}\) topology, but may support two robust Dirac points on highsymmetry surface facets exhibiting additional crystalline symmetries. For example, the (111) facet has \({\hat{C}}_{3}\) rotation symmetry; the two Dirac points are located at the Tpoint and belong to different \({\hat{C}}_{3}\) eigenvalue sectors having \({\hat{C}}_{3}\) eigenvalues −1 and \(\exp (\pm {\mathrm{i}}\pi /3)\) respectively^{1}. If the two Dirac points are pinned at the same energy, then they cannot be gapped out while preserving the \({\hat{C}}_{3}\) (no intercone gap) and timereversal symmetries (no intracone gap). However, there are no symmetry constraints that fix the energies of the two cones, and generically it is expected that the (111) surface will be gapped^{1}. In this context, ref. ^{1} considered the case where the (111) facet is the top facet of a hexagonal crystal (as shown in Fig. 1a). For this geometry, the \({\hat{C}}_{3}\) symmetry and timereversal symmetry are compatible with signalternating surfacestate masses/gaps on the side facets (this breaks \({\hat{C}}_{6}\) but preserves \({\hat{C}}_{3}\))^{1}. Since the surface Dirac cones on the top/bottom (111) facets can also be generically gapped while preserving the symmetries, this will lead to sharply localized hinge modes where the side surfaces intersect the top/bottom surfaces, which were first observed for bulk Bi crystals in refs. ^{1,17}, and confirmed for Bi films in our measurements above.
We propose that the observed edge states of an island on the (110) surface can be ascribed to \({\hat{C}}_{2}\) (of the bulk crystal around the \((1\bar{1}0)\) axis) and timereversal symmetry protected higherorder topology consistent with ref. ^{18}. The (110) surfaces of our islands do not have any protective crystal symmetry and thus we generically expect the two surface Dirac cones on those surfaces (as predicted by ref. ^{18}) to be gapped. When considering hinge states though, we must also consider the mass gaps for surface states on the sidesurfaces of such islands. First, the two long sides/edges of the (110) rectangular islands do not have any protected crystal symmetry, hence we expect the surface states to be gapped. Second, the two short sides/edges of the (110) rectangular islands are truncated (\(1\bar{1}0\)) surfaces, which could show remnants of the two gapless Dirac cone surface states. Indeed, ref. ^{18} recently emphasized that the (\(1\bar{1}0\)) surface has \({\hat{C}}_{2}\) rotation symmetry that protects the two, generically unpinned, surface Dirac points related by \({\hat{C}}_{2}\) rotation. In this case, the (\(1\bar{1}0\)) facet, cannot be gapped out (perturbatively) as long as the \({\hat{C}}_{2}\) and timereversal symmetries are preserved since the Dirac cones do not coincide at a TRIM. However, since we are considering a surface island, translation symmetry is strongly broken on the (\(1\bar{1}0\)) facets. Hence, we do not expect the surface states to be robust since their momentum space locations become irrelevant. From these arguments, we expect that the surfaces that form the top and sides of the island can be generically gapped, so we can explore our observations in the context of higherorder topology in this system. In contrast to previous systems with crystallineprotected topology, (e.g., the mirrorprotected surface Dirac cones in SnTe^{25}), the (110) surface of Bi does not preserve the \({\hat{C}}_{2}\) bulk symmetry responsible for the higherorder protection^{4}. However, this does not mean that we cannot observe signatures of higherorder topology, it just implies that the possible hinge state patterns may be affected by the details of the surface termination. For a rectangular crystal, as shown in Fig. 3f, where (\(1\bar{1}0\)) is the top edge/facet, there are two inequivalent configurations of surface mass gaps that match our observations of hinge modes on the (110) facet; i.e., that helical modes are localized on only three edges out of four. The configuration of helical hinge modes shown in the left panel of Fig. 3f nominally preserves both \({\hat{C}}_{2}\) (on the (\(1\bar{1}0\)) surface termination) and timereversal symmetries, while the configuration shown in the right panel of Fig. 3f preserves only the timereversal symmetry (details can be found in Supplementary Note 2). In addition, both configurations of helical hinge modes in Fig. 3f that are consistent with our observations, require broken inversion symmetry on the surface termination (which is a symmetry of the bulk of a bismuth crystal). However, this is not problematic since inversion is naturally broken for an island on a surface. Thus, we find that our observations corroborate, and are clearly indicative of higherorder topology in bismuth.
Spectroscopic measurements on Bi_{0.92}Sb_{0.08}(110)
We can now use our established signature of higherorder topology in Bi to determine the topological nature of Bi alloyed with Sb. Previous theoretical studies have suggested that the Bi_{1−x}Sb_{x} alloy undergoes a trivialtotopological bandinversion transition at approximately x = 0.04^{26,27,28}. However, similar to Bi, the narrow band gaps and the existence of multiple bulks and surface bands near the Fermi energy have made the theoretical and experimental determination of the topological properties of Bi_{1−x}Sb_{x} complicated. From our studies on Bi, we propose that the pattern of the edge modes on the (110) oriented rectangular islands may provide a clear picture of the topology in this compound. Figure 4b shows STM spectra at an edge and plateau of the (110) facet of Bi_{0.92}Sb_{0.08}. A peak centered around 100 meV is observed at the edge, similar to that observed on Bi islands. Spectroscopic measurements across and along the edge shown in Fig. 4c, d respectively, reveal that this mode is localized to the edge. Importantly, similar to our data on Bi, we observe edge modes on three out of the four edges of the (110) oriented rectangular islands as shown in Fig. 4f−i. The explanation of this pattern of edge modes requires the system to be higherorder, and hence requires that the bulk has a trivial strong \({{\mathbb{Z}}}_{2}\) topology. Hence, our data on Bi_{0.92}Sb_{0.08} suggests that it has a trivial strong \({{\mathbb{Z}}}_{2}\) topology and falls in the HOTI regime. This bears further study using other experimental techniques since it calls into question some longaccepted predictions about BiSb alloys, and indeed may have implications for the celebrated identification of nearby Bi_{0.9}Sb_{0.1} as a strong \({{\mathbb{Z}}}_{2}\) topological insulator.
Discussion
In summary, we have studied (110) oriented Bi and Bi_{0.92}Sb_{0.08} films with STM and STS. We observe bound modes on three out of four edges of a rectangular island on (110) facets. Moreover, the edge showing no edge modes is always perpendicular to the (\(1\bar{1}0\)) direction. Theoretically, the novel pattern of the metallic edge modes observed on the (110) facets can be explained by a higherorder topology protected by timereversal (\(\hat{T}\)) symmetry and bulk twofold rotation (\({\hat{C}}_{2}\)) symmetry around the (\(1\bar{1}0\))axis^{18}. Based on this we confirm that Bi and Bi_{0.92}Sb_{0.08} belong to the HOTI class of topological materials. The latter result is particularly interesting since previous theoretical studies indicate that Bi_{1−x}Sb_{x} with x ~ 0.08 should already be in a strong \({{\mathbb{Z}}}_{2}\) topological insulator phase heralded by a band inversion predicted at x ~ 0.04^{26,27,28}. Our work brings new insights to the topology of Bi_{0.92}Sb_{0.08} which is revealed as a new HOTI.
Methods
Sample preparation
Highly crystalline films of Bi and Bi_{0.92}Sb_{0.08} were grown on ndoped silicon (111) wafers using a custom ultrahigh vacuum molecular beam epitaxy system. Before deposition, Si substrates were cleaned by ultrasonication in acetone and isopropanol. The substrates were then transferred to the MBE system (pressure < 2 × 10^{−9} Torr) and degassed at 520 ^{∘}C for 10−12 h. After degassing, the substrate was cleaned by flash annealing, where they were repeatedly heated from 650 to 900 ^{∘}C in 80 s. Each cycle helps to remove oxide layers or impurities from the silicon surface. The surface quality was confirmed by the observation of clear 7 × 7 reconstructed RHEED patterns. The substrate was rapidly cooled from 650 ^{∘}C to room temperature at the rate of 1−2 ^{∘}C/s after 16 cycles of flash annealing. For film growth, bismuth (purity ~ 99.9999%) and antimony (purity ~ 99.9999%) sources were evaporated from standard Knudcell cells at flux rates 0.0769 and 0.0071 Å/s respectively, as measured by a Quartz Crystal monitor. The substrates were held at room temperature during growth.
STM measurements
Samples were transferred from MBE chamber to a vacuum suitcase at pressure < 3 × 10^{−10} and subsequently transferred to a Unisoku UHVSTM without exposure to air. All the measurements were done at 4.3 K. Normal tungsten tips were prepared by the etching method and used after cleaning by electron beam heating. All the topographic images were taken in constantcurrent mode and spectroscopic signals were recorded by standard lockin amplifier with ac modulation 3−3.5 mV at 983 Hz frequency.
Data availability
The relevant datasets will be made available from the corresponding authors on reasonable request.
References
Schindler, F. et al. Higherorder topology in bismuth. Nat. Phys. 14, 918 (2018).
Song, Z., Fang, Z. & Fang, C. (d2)dimensional edge states of rotation symmetry protected topological states. Phys. Rev. Lett. 119, 246402 (2017).
Benalcazar, W. A., Bernevig, B. A. & Hughes, T. L. Electric multipole moments, topological multipole moment pumping, and chiral hinge states in crystalline insulators. Phys. Rev. B 96, 245115 (2017).
Schindler, F.et al. Higherorder topological insulators. Sci. Adv. 4, eaat0346 (2018).
Olsen, T., Rauch, Tcv, Vanderbilt, D. & Souza, I. Gapless hinge states from adiabatic pumping of axion coupling. Phys. Rev. B 102, 035166 (2020).
Zhu, P., Hughes, T. L. & Alexandradinata, A. Quantized surface magnetism and higherorder topology: application to the Hopf insulator. Phys. Rev. B 103, 014417 (2021).
SerraGarcia, M. et al. Observation of a phononic quadrupole topological insulator. Nature 555, 342–345 (2018).
Peterson, C. W., Benalcazar, W. A., Hughes, T. L. & Bahl, G. A quantized microwave quadrupole insulator with topologically protected corner states. Nature 555, 346–350 (2018).
Noh, J. et al. Topological protection of photonic midgap defect modes. Nat. Photonics 12, 408–415 (2018).
Imhof, S. et al. Topolectricalcircuit realization of topological corner modes. Nat. Phys. 14, 925–929 (2018).
Choi, Y.B. et al. Evidence of higherorder topology in multilayer WTe_{2} from Josephson coupling through anisotropic hinge states. Nat. Mater. 19, 974–979 (2020).
Lee, E., Kim, R., Ahn, J. & Yang, B.J. Twodimensional higherorder topology in monolayer graphdiyne. npj Quantum Mater. 5, 1–7 (2020).
Zhang, R.X., Wu, F. & Sarma, S. D. Möbius insulator and higherorder topology in MnBi_{2n}Te_{3n+1}. Phys. Rev. Lett. 124, 136407 (2020).
Wang, Z., Wieder, B. J., Li, J., Yan, B. & Bernevig, B. A. Higherorder topology, monopole nodal lines, and the origin of large Fermi arcs in transition metal dichalcogenides XTe_{2}(X = Mo, W). Phys. Rev. Lett. 123, 186401 (2019).
Zhang, R.X., Cole, W. S., Wu, X. & Sarma, S. D. Higherorder topology and nodal topological superconductivity in Fe(Se,Te) heterostructures. Phys. Rev. Lett. 123, 167001 (2019).
Park, M. J., Kim, Y., Cho, G. Y. & Lee, S. Higherorder topological insulator in twisted bilayer graphene. Phys. Rev. Lett. 123, 216803 (2019).
Drozdov, I. K. et al. Onedimensional topological edge states of bismuth bilayers. Nat. Phys. 10, 664–669 (2014).
Hsu, C.H. et al. Topology on a new facet of bismuth. Proc. Natl Acad. Sci. USA 116, 13255–13259 (2019).
Takayama, A., Sato, T., Souma, S., Oguchi, T. & Takahashi, T. Onedimensional edge states with giant spin splitting in a bismuth thin film. Phys. Rev. Lett. 114, 066402 (2015).
Kawakami, N., Lin, C.L., Kawai, M., Arafune, R. & Takagi, N. Onedimensional edge state of Bi thin film grown on Si (111). Appl. Phys. Lett. 107, 031602 (2015).
Nagao, T. et al. Nanofilm allotrope and phase transformation of ultrathin bi film on Si(111) −7 × 7. Phys. Rev. Lett. 93, 105501 (2004).
Kokubo, I., Yoshiike, Y., Nakatsuji, K. & Hirayama, H. Ultrathin Bi(110) films on \({\rm{Si}}(111)\sqrt{3}\times \sqrt{3}{\rm{B}}\) substrates. Phys. Rev. B 91, 075429 (2015).
Nagase, K., Ushioda, R., Nakatsuji, K., Shirasawa, T. & Hirayama, H. Growth of extremely flat Bi(110) films on a \({\rm{Si}}(111)\sqrt{3}\times \sqrt{3}{\rm{B}}\) substrate. Appl. Phys. Express 13, 085506 (2020).
Takayama, A., Sato, T., Souma, S. & Takahashi, T. Rashba effect in antimony and bismuth studied by spinresolved arpes. N. J. Phys. 16, 055004 (2014).
Tanaka, Y. et al. Experimental realization of a topological crystalline insulator in SnTe. Nat. Phys. 8, 800–803 (2012).
Lenoir, B.et al. Bisb alloys: an update. In Fifteenth International Conference on Thermoelectrics. Proceedings ICT’96 1−13 (IEEE, 1996).
Fu, L., Kane, C. L. & Mele, E. J. Topological insulators in three dimensions. Phys. Rev. Lett. 98, 106803 (2007).
Teo, J. C., Fu, L. & Kane, C. Surface states and topological invariants in threedimensional topological insulators: application to Bi_{1−x}Sb_{x}. Phys. Rev. B 78, 045426 (2008).
Acknowledgements
STM studies and theoretical work at the University of Illinois, UrbanaChampaign were primarily supported by the Materials Research Science and Engineering Center DMR1720633. V.M. acknowledges support from the Gordon and Betty Moore Foundation’s EPiQS Initiative, Grant GBMF9465 for MBE growth and characterization. The authors thank Guannan Chen, Zhuozhen Cai, Yulia Maximenko and Charlie Steiner for valuable discussions. Thinfilm characterization was carried out in part in the Materials Research Laboratory Central Research Facilities at the University of Illinois.
Author information
Authors and Affiliations
Contributions
T. L. H and V. M. conceived the idea, designed the experiments, and developed the analysis tools. L. A. grew and characterized all the materials and carried out the STM/STS experiments. P. Z. carried out the theoretical analysis. V. M. and T. L. H supervised all aspects of the project. All authors jointly wrote the paper.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Peer review information Nature Communications thanks Jian Li and the other, anonymous, reviewer(s) for their contribution to the peer review of this work.
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Aggarwal, L., Zhu, P., Hughes, T.L. et al. Evidence for higher order topology in Bi and Bi_{0.92}Sb_{0.08}. Nat Commun 12, 4420 (2021). https://doi.org/10.1038/s41467021246838
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41467021246838
This article is cited by

Theoretical studies of magnetooptical Kerr and Faraday effects in twodimensional secondorder topological insulators
Scientific Reports (2023)

Longlived Andreev states as evidence for protected hinge modes in a bismuth nanoring Josephson junction
Nature Physics (2023)

Spincharge separation and quantum spin Hall effect of \(\beta\)bismuthene
Scientific Reports (2023)

Bulkboundarytransport correspondence of the secondorder topological insulators
Science China Physics, Mechanics & Astronomy (2023)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.